Gel permeation chromatography (GPC) has become the most widely used technique for analyzing polymer samples in order to determine their molecular weights and weight distributions. Examples of GPC chromatograms of polystyrene samples with their molecular weights and dispersities are shown on the left.
  Benoit and co-workers proposed that the hydrodynamic volume, V, which is proportional to the product of [η] and M, where [η] is the intrinsic viscosity of the polymer in the SEC eluent, may be used as the universal calibration parameter. If the Mark–Houwink–Sakurada constants K and α are known (see Mark–Houwink equation), a plot of log [η]M versus elution volume (or elution time) for a particular solvent, column and instrument provides a universal calibration curve which can be used for any polymer in that solvent. By determining the retention volumes (or times) of monodisperse polymer standards (e.g. solutions of monodispersed polystyrene in THF), a calibration curve can be obtained by plotting the logarithm of the molecular weight versus the retention time or volume. Once the calibration curve is obtained, the gel permeation chromatogram of any other polymer can be obtained in the same solvent and the molecular weights (usually M and M) and the complete molecular weight distribution for the polymer can be determined. A typical calibration curve is shown to the right and the molecular weight from an unknown sample can be obtained from the calibration curve.